J. Cell. Mol. Med. Vol 10, No 1, 2006 pp. 7-19
Tissue engineering of bone:
the reconstructive surgeon's point of view
U. Kneser a *, D.J. Schaefer b, E. Polykandriotis a, R.E. Horch a
a Department of Plastic and Hand Surgery, University of Erlangen Medical Center, Erlangen, Germany
b Department of Plastic, Reconstrucitive and Aesthetic Surgery, Clinic of Reconstructive Surgery,
University Hostpital Basel, Basel, Switzerland
Received: January 17, 2006; Accepted: February 6, 2006
Bone defects represent a medical and socioeconomic challenge. Different types of biomaterials are applied for recon-
structive indications and receive rising interest. However, autologous bone grafts are still considered as the gold standard
for reconstruction of extended bone defects. The generation of bioartificial bone tissues may help to overcome the prob-
lems related to donor site morbidity and size limitations. Tissue engineering is, according to its historic definition, an
"interdisciplinary field that applies the principles of engineering and the life sciences toward the development of biolog-
ical substitutes that restore, maintain, or improve tissue function". It is based on the understanding of tissue formation and
regeneration and aims to rather grow new functional tissues than to build new spare parts. While reconstruction of small
to moderate sized bone defects using engineered bone tissues is technically feasible, and some of the currently developed
concepts may represent alternatives to autologous bone grafts for certain clinical conditions, the reconstruction of large-
volume defects remains challenging. Therefore vascularization concepts gain on interest and the combination of tissue
engineering approaches with flap prefabrication techniques may eventually allow application of bone-tissue substitutes
grown in vivo with the advantage of minimal donor site morbidity as compared to conventional vascularized bone grafts.
The scope of this review is the introduction of basic principles and different components of engineered bioartificial bone
tissues with a strong focus on clinical applications in reconstructive surgery. Concepts for the induction of axial vascu-
larization in engineered bone tissues as well as potential clinical applications are discussed in detail.
Keywords: tissue engineering • bone replacement • vascularization • flap prefabrication • microsurgery • AV loop
* Correspondence to: Ulrich KNESER, M.D.
Department of Plastic and Hand Surgery,
University of Erlangen Medical Center,
Krankenhausstrasse 12, 91054 Erlangen Germany.
Tissue Engineering Review Series Guest Editor: R.E. Horch
– Function and structure of bone
– Components of bone tissue
– Bone regeneration
• Established treatment of bone defects
– Bone grafts
– Osteoinductive substances
• Tissue engineering
– Basic principles
– Properties of bioartificial bone tissues
• Components of bioartificial bone tissues
– Osteogenic cells
– Osteoinductive factors and gene transfer
• Vascularization of engineered bone tissues
– Angioinductive growth factors
– Endothelial cells
– Local factors at the recipient site
• Surgical angiogenesis
– Flap prefabrication and bone grafts
– Generation of vascularized bioartificial
– "Free-style" vascularized bioartificial
Available online at
the CMM Foundation
Journal of Cellular and Molecular Medicine
Function and structure of bone
Bone is a dynamic, highly vascularized tissue with
the unique capacity to heal and remodel without leav-
ing a scar [1, 2]. It provides mechanical stability to the
skeleton that is needed for load bearing, locomotion
and protection of internal organs. Furthermore bone
serves as a mineral reservoir and has the capacity to
rapidly mobilize mineral stores if needed for home-
ostasis of the calcium blood level. The diversity of
functional requirements of bone tissue is reflected by
its complex architecture. In the adult skeleton bone
tissue is either arranged in a trabecular pattern (can-
cellous bone) or in a compact pattern (cortical bone)
. Cortical bone is almost solid with less than 10%
porosity and ubiquitously present in long, short and
flat bones. In contrast, cancellous bone is organized in
a porous sponge-like pattern. This type of bone har-
bors a large part of the bone marrow and is essential-
ly present in the metaphysis of long bones, the iliac
crest and the vertebral bodies .
Components of bone tissue
Although bone tissue is populated by a variety of dif-
ferent cells, its functional integrity is maintained by
three different cell types: osteoblasts, osteocytes and
osteoclasts [2, 4, 5]. These tissue-specific cells are
embedded in a highly complex matrix that consists of
a mineralized (hydroxylapatite) and a non-mineral-
ized component [6, 7]. The non-mineralized, organic
part contains collagens, glycoproteins, proteoglycans
and sialoproteins that play an essential role in control
of growth and differentiation of osteoblasts, osteo-
cytes and osteoclasts and in bone remodeling [7–10].
Bone development and bone regeneration are com-
plexly regulated processes that involve a plethora of
different growth and transcription factors which coor-
dinate the interaction of cells and matrix in response
to external or internal stimuli [9, 11–20].
Bone regeneration is a highly efficient and tightly
regulated process that involves all the above-men-
tioned components of bone tissue. Bone regenera-
tion is the result of a continuous interplay between
growth factors and cytokines for both initiation and
regulation of the remodeling process. [7, 17, 21].
The majority of fractures heal well under standard
conservative or surgical therapy. However, extend-
ed bone defects following trauma or cancer resec-
tion or non-unions of fractures may require more
sophisticated treatment. In these cases bone graft-
ing procedures, segmental bone transport, distrac-
tion osteogenesis or biomaterials are applied for
Established treatment of bone defects
Today, autologous bone grafting is the gold stan-
dard for osteogenic bone replacement in osseous
defects . Autologous bone grafts reliably fill
substance deficits and induce bone tissue formation
at the defect site following transplantation. These
grafts exhibit, depending on donor site, size, shape
and quality, some initial stability. Chips, larger
pieces and even blocks of several centimeters in
size could be harvested. The use of other types of
bone substitutes in combination with autologous
bone grafts decreases the amount of bone tissue
needed for reconstruction . However, the clini-
cal use of autologous osseous transplants is limited
by a considerable donor site morbidity that increas-
es with the amount of harvested bone. Bleeding,
hematoma, infection, and chronic pain are common
complications of bone graft harvest [28–30].
Processed allogenic or xenogenic bone grafts are
also commonly used for repair of osseous defects
when autologous transplantation is not applicable
[26, 31–33]. Although the initial properties of allo-
genic or xenogenic grafts resemble those of autolo-
gous bone in terms of biomechanic stability and
elasticity, the lack of osteogenicity represents a lim-
itation even when osteoinductive factors are pre-
served during processing.
For specific indications vascularized bone grafts
from different locations such as fibula, scapula,
iliac crest and others are taken and transplanted into
given bone defects using microsurgical techniques
[34-36]. Large tissue defects with exposed struc-
tures like, bones, joints, tendons and nerves in
regions of compromised perfusion do require a tis-
sue transplant which brings good vascularity into
the affected zone and positively affects healing in
the broader sense of the nutrient flap. However, free
bone tissue transfer is associated with donor site
morbidity . Furthermore, availability is limited
in quality and quantity.
A variety of different biomaterials is currently
being used for reconstruction of bone defects.
Acrylate-based bone cements provide, after poly-
merization a high mechanical stability [38, 39].
They are widely used for fixation of total joint
prosthesis, vertebroplasty and for craniofacial
bone defects; they may be loaded with antibiotics
for local drug delivery. However, despite sophisti-
cated modes of application they do not possess
osteogenic or osteoinductive properties and are,
when at all, slowly resorbed. The long-term inte-
gration of non-porous bone cements into bone
defects is not always warranted. Within the last
two decades, many other biogenic and synthetic
materials were evaluated for their use as bone sub-
stitutes. Calcium phosphate- and apatite-based
bone cements, porous composites as well as other
types of biomaterials have been clinically applied
for treatment of fractures and bone defects
[40–42]. They are, depending on their chemical
composition and porosity osteoconductive,
biodegradable and are integrated into given bone
defects. However, in general terms their biome-
chanic stability is significantly lower in compari-
son to acrylate-based implants.
Although osteoinductive substances are clinically
applied for reconstruction of bone defects or for
acceleration of fracture healing, only small num-
bers of patients have been treated and application
modes and indications are not completely stan-
dardized yet. Platelet rich plasma contains, besides
platelet derived growth factor (PDGF), depending
on processing and application modes, a variety of
different growth factors [43–45]. It enhanced bone
formation in experimental and clinical settings.
Demineralized bone matrix (DBM) is prepared
from allogenic or xenogenic bone and commercial-
ly available for clinical application in different for-
mulations [46–49]. Its osteoinductive potential is
highly variable and depends not only on the donor
but also on the processing protocols. DBM is com-
monly used in combination with other types of bio-
materials . Bone morphogenetic proteins
(BMPs) have been identified as the most relevant
osteoinductive factor in demineralized bone matrix
[17, 51]. Right now there are two types of BMPs
being clinically applied  [53–55]. Application
of BMP 2 in open tibial fractures significantly
improved bone healing in comparison to a conven-
tionally treated control group in a randomized
study . However, heterotopic ossification, sub-
optimal release kinetics, and last but not least the
high price pose a challenge to widespread applica-
tion of these substances.
Tissue Engineering is a young field of research.
Initially, it was defined as “… an interdisciplinary
field that applies the principles of engineering and
the life sciences toward the development of biolog-
ical substitutes that restore, maintain, or improve
tissue function” . Tissue Engineering is based
on the profound understanding of embryology, tis-
sue formation and regeneration and aims to grow-
ing new functional tissues rather than building new
spare parts. As mentioned above, it combines inte-
gral knowledge from physicists, chemists, engi-
neers, material scientists, biologists and physicians
to a comprehensive interdisciplinary approach.
Tissue Engineering is tightly associated with the
field of regenerative medicine.
How to grow new tissues? Independent of the type of
tissue, cells, extracellular matrix, blood vessels,
nerves, intercellular communication and cell-matrix
interaction are only some “ingredients” to grow new
tissues in vivo. These single components have to be
combined in a well coordinated spatial and time
dependent fashion. Besides the above-mentioned
“ingredients”, well elaborated surgical concepts are a
prerequisite for successful in vivo application of tissue
engineering concepts. Caution is needed with increas-
J. Cell. Mol. Med. Vol 10, No 1, 2006
ing complexity of the engineered tissue composites, to
prevent damage of the susceptible cells or bioactive
substances during implantation. Depending on the
specific concept, a facultative in vitro period prior to
implantation may vary from 1 day up to several
months. This period is commonly used for cell expan-
sion or induction of tissue-specific cell differentiation.
In the experimental setting Tissue Engineering con-
cepts have been successfully applied to generate many
different types of tissues such as bone, cartilage, liver,
muscle, skin and others [57–62].
Properties of bioartificial bone tissues
The intended clinical use defines the desired proper-
ties of engineered bone substitutes. Defects of load-
bearing long bones, for instance, require constructs
with high mechanic stability whereas initial plastic-
ity is not essential. On the other hand for craniofa-
cial applications, initially injectable or moldable
constructs are favorable. Although stable integration
of the implants is imperative, the mechanic loads
involved are not as high as in the former situation.
Depending on the implantation site, initial vascular-
ization may be essential for enhanced engraftment
and prevention of infections. Mechanical stability,
osteoconductivity (i.e. the capacity of a material to
guide bone forming tissue into a defect ),
osteoinductivity (i.e. the ability to induce bone for-
mation by attracting and stimulating bone-forming
cells of the recipient ), osteogenicity (i.e. the
capability to form bone tissue de novo ), and
ease of handling have to be well balanced in order to
properly meet the clinician’s needs.
Components of bioartificial bone
Any vital tissue consists of matrix and cells. The
matrix acts as a biological three-dimensional scaf-
fold for cells within tissues and provides cells with
the tissue-specific environment and architecture
. Physiologically it serves as a reservoir for
water, nutrients, cytokines and growth factors and
allows cells to attach to it. For tissue engineering
purposes, three main components could be extract-
ed from this complex network of different intercon-
nected functions: Mechanic support, cell attach-
ment and participation in cellular communication
pathways. A vast variety of materials has been used
as matrix for bone tissue engineering applications
[66, 67]. Porosity, surface chemistry, topography,
three-dimensional architecture, immunogenicity
and mechanic parameters are matrix properties
which significantly influence formation of bone
within bioartificial bone substitutes . Gel-like
matrices such as fibrin have been used for cell
immobilization in combination with other scaffolds
. While a variety of highly innovative matrices
are under in vitro and in vivo evaluation, clinically
established and approved biomaterials are readily
available for first applications of bioartificial bone
tissues [70–77]. Computer assisted design – com-
puter assisted manufacturing (CAD/CAM) and
rapid prototyping techniques allow the generation
of custom-made scaffolds for cell delivery that fit
into certain bone defects [77, 78].
Osteogenic cells are an integral part of any tissue
engineering strategy. These cells are either trans-
planted along with the appropriate scaffolds into the
bone defect or attracted from the host by osteoin-
ductive factors. Osteogenic cells are not a homoge-
nous cell population. A differentiation pathway sim-
ilar to that of hematopoetic cells has been postulat-
ed [79, 80]. The affectors of bone remodeling,
regeneration and fracture repair in the adult organ-
ism are the cellular components. Today it is still
unknown which type of osteogenic cell will be the
one most suitable for engineering of bone tissue.
Mesenchymal stem cells, Bone marrow stromal
cells, periosteal cells and osteoblasts have been suc-
cessfully used for the generation of bone tissue [4,
75, 76, 81–83]. Isolation and expansion efficiency,
stability of osteoblastic phenotype, in vivo bone for-
mation capacity, and long-term safety are essential
requirements that have to be met by any type of
osteogenic cell for successful clinical application.
Serum-free culture conditions or culture medium
supplemented with autologous serum are preferable
for cell expansion in vitro.
Recently, clinical applications of tissue engi-
neered bone have been reported. Quarto et al. treated
three patients with large bone defects of the tibia,
ulna, and humerus, using macro porous hydroxyap-
atite scaffolds seeded with autologous in vitro
expanded bone marrow stromal cells immobilized in
collagen gel. All patients recovered limb function
without major complications. Vacanti and coworkers
reconstructed a patient’s thumb using periosteal cells
and a coral-based hydroxyl apatite scaffold .
Although the patient did well after implantation and
hand function recovered significantly, quantitative
histomorphometric analysis of a biopsy revealed that
eventually only 5% of the implant volume was bone.
The outcome of this clinical trial was not superior to
that of conventional reconstructive approaches .
Periosteal cell-seeded polymer fleeces or mesenchy-
mal stem cells and platelet-rich plasma, immobilized
in beta-tricalcium phosphate scaffolds induced bone
formation in sinus lift operations [86–88]. Despite
anecdotal reports of successful implantation of engi-
neered bone tissues, the small number of patients
makes it difficult to eventually assess the efficacy of
these constructs and comparison with conventional
methods has not been performed yet.
Osteoinductive factors and gene transfer
Osteogenic substances augment the osteogenic
capacity of tissue engineered bone constructs. They
are either applied as a crude and hardly standardized
mixture of proteins as described above (demineral-
ized bone matrix and platelet rich plasma) or as iso-
lated factors [21, 44, 47]. Osteoinductive growth fac-
tors have the capability to modulate proliferation and
differentiation of implanted osteogenic cells.
Furthermore these substances are able to attract pre-
cursor cells from the host to invade scaffold and
induce osteoblastic differentiation. There is a large
number of such proteins that stimulate proliferation
and/or differentiation of osteogenic cells in vitro and
in vivo. Some osteogenic factors have been cloned
and are commercially available as recombinant pro-
teins. Bone morphogenetic proteins (BMPs) are upon
the most potent osteoinductive factors. BMPs belong
to the TGF-β family and bind to extracellular matrix
components such as heparan sulfate and type IV col-
lagen [89, 90]. BMP2 and BMP-7 are being clinical-
ly applied for fractures and non-unions, but only a
limited number of patients have been treated so far
with long term follow up still pending [54, 55]. The
effective in vivo use of isolated osteoinductive growth
factors requires optimized pharmacokinetics.
Intelligent delivery systems have proven to be of cru-
cial importance for reliable bone formation and eco-
nomic application of BMPs . Without controlled
release systems, growth factors rapidly diffuse away
from the constructs.
Gene therapeutic approaches potentially promote
pertinent function of osteogenic cells and enhance
performance of bioartificial bone tissues [92-95].
Expression systems for osteoinductive growth fac-
tors are therefore of high interest. There are different
strategies to bring DNA sequences into cells. Viral
vectors provide high transfection efficiency and
some viruses even allow stable transfection of
osteogenic cells . Clinical use in tissue engineer-
ing concepts is however hampered by safety con-
cerns. Non-viral gene transfer is achieved by either
using transfection reagents, or by mediator-free tech-
niques . Matrix-mediated gene transfer is anoth-
er innovative approach that avoids the use of any
transfection reagent or potentially harmful vector
. In conclusion, gene transfer strategies may pro-
vide for efficient stimulation of bone formation with-
in bioartificial bone tissues, but further insight into
long-term effects, phenotypical stability and applica-
tion techniques need to precede any wide-spread
application in humans.
Vascularization of engineered bone
Adequate vascularization is a prerequisite for for-
mation of high quality bone. When in vitro engi-
neered cellular constructs are transferred in vivo
they have to rely on processes like interstitial
fluid diffusion and blood perfusion. Here recites a
core limitation for transfer of tissue engineering
models from the in vitro to the in vivo environ-
ment. Diffusion is the initial process involved, but
it can only provide for cell support within a max-
imum range of 200 µm into the matrix [99, 100].
The survival of cells in the center of large cell-
containing constructs is therefore often limited by
suboptimal initial vascularization . Cell label-
ing experiments disclosed a considerable loss of
osteoblasts within the first week following trans-
plantation in porous cancellous bone matrices
. For this reason induction of vascularization
is an integral element of any successful bone tis-
sue engineering concept.
J. Cell. Mol. Med. Vol 10, No 1, 2006
Angioinductive growth factors
Angiogenesis is a complexly regulated process
[102–104]. Several mechanisms of regulation are
involved throughout the angiogenetic cascade of events;
the endothelial cell acting as the main mediator of neo-
vascular growth is guided through space and time. A
large number of angiogenic factors work together in a
highly coordinated manner to induce endothelial cell
factors are promising tools for induction and accelera-
tion of vascularization processes in three-dimensional
scaffolds [105, 106]. VEGF and bFGF have been suc-
cessfully used to improve vascularization of engineered
tissues . Immobilization of angiogenetic growth
factors, for instance in fibrin gels or by using heparine-
binding release systems, allows for optimized release
kinetics and longer lasting effects [108, 109].
Endothelial cells, either derived from microvascula-
ture, umbilical veins or large blood vessels, have been
used for generation of capillary-like structures and
vessles in vitro by different groups [110–112]. In vivo
these cells are supposed to form networks of capillar-
ies and gain access to the recipient’s circulation .
Although the newly formed vascular networks dis-
play, depending on the experimental setting, a differ-
entiated morphology, the processes that occur upon
implantation are not completely understood at the
moment and there are only scarce in vivo data on the
efficiency of this approach with regard to enhance
and accelerate vascularization of bioartificial tissues.
Since cell-containing constructs require immediate
supply with nutrients and oxygen after implantation
and even with synchronous transplantation of
endothelial cells some time is needed for formation of
anastomoses between newly formed capillaries and
the recipient’s circulation, the potential benefits of
endothelial cell transplantation for induction of vas-
cularization are questionable .
Local factors at the recipient site
Local factors play a prominent role in tissue engi-
neering concepts since the quality of the tissue at the
recipient site influences vascularization of the scaf-
folds, cell engraftment and eventually bone forma-
tion. Neovascularization from the surrounding tis-
sues, which is responsible for long-term survival of
transplanted osteogenic cells, is a slow process so
that constructs pre-seeded with tissue specific cells
need to be sufficiently thin to ensure rapid vascular-
ization and cell survival . Even a perfectly engi-
neered piece of tissue will fail to form bone when the
local environment is inappropriate. In a clinical set-
ting, for instance in cases of large bone defects fol-
lowing trauma or osteomyelitis, bacterial load and
chronic scarring pose even more challenge to the
transplanted constructs. Plastic surgical concepts
may help to bridge the gap between perfectly in vitro
engineered bone tissues and the sometimes disap-
pointing in vivo performance.
The majority of the above-mentioned tissue engineer-
ing approaches rely on the so called “extrinsic” mode
of neovascularization . The neovascular bed
originates from the periphery of the construct which
should be implanted into a site of high vascularization
potential. Subcutaneous , intramuscular ,
and intraperitoneal  implantation has been report-
ed.Although generation of vascularized bone tissue is
feasible using this technique, this tissue is vascular-
ized in a random pattern. Transfer to distant implan-
tation sites is impossible without destruction of the
vascular network. Reconstructive surgeons aim there-
fore to generate so called “axially vascularized” tis-
sues that could be transferred to the defect site using
microsurgical techniques of vascular anastomosis.
These tissues are immediately vascularized upon
implantation into the defect as free flaps do. In the
following section different techniques for the induc-
tion of axial vascularization in bone grafts are dis-
cussed in detail.
Flap prefabrication and bone grafts
Conventional osteomyocutaneous flaps do not
always meet the requirements of a composite
defect. A prefabricated composite flap can be cre-
ated according to the complex geometry of the
defect. Prefabrication of multi component flaps is a
well established procedure in plastic surgery
[118–120]. This concept is based on the revascu-
larization phenomenon directly related to host tis-
sue vascularity  and significantly expanded
the frontiers of reconstructive surgery. Tissue pre-
fabrication is essentially a method comprised by
two steps. During the first procedure a tissue com-
ponent is formed into the wanted shape and is
thereupon implanted into a region with a vascular
axis suitable for microsurgical transfer. During the
second stage the autologous implant is harvested
en-bloc with the surrounding tissue and the vascu-
lar pedicle as a free flap. The implant acquires its
vascularization from the tissue block and the flap is
connected to the local circulation by means of a
Prefabrication allows the transfer of preferred tis-
sue composites suitable for reconstruction regard-
less of their native vascular origin as free or pedicled
flaps and helps to reduce donor site morbidity .
Prefabrication of bone flaps using plastic surgical
techniques may help to circumvent preceding prob-
lems of microsurgical bone transfer and to obtain
previously non-existing tissue units that meet exact-
ly the specific recipient site needs. Basically there
are two strategies for flap prefabrication: either a
bone graft is wrapped in axially vascularized tissues
(cutaneous, fascioucutaneous or muscle flaps) or a
vascular axis is implanted into the bone graft. The
latter type of vascularization is called “intrinsic”. In
the “intrinsic” mode of vascularization the construct
acquires an inherent perfusion and does not have to
rely on favourable local conditions. This is achieved
by inducing angiogenesis from a centrally located
vascular axis. The configuration of the vascular axis
could vary according to the reconstructive require-
ments . After a facultative vascularization peri-
od the vascularized graft is transferred into the bone
defect using conventional or microsurgical tech-
niques. Prefabricated bone grafts have been clinical-
ly applied in different settings [124, 125].
Generation of vascularized bioartificial
Flap prefabrication using conventional bone grafts
allows generation of new types of flaps indepen-
dent of the vascular anatomy of the bone trans-
plant. However, the donor site morbidity after har-
vesting of the bone grafts is still a problem.
Recently, biomaterials, osteogenic cells and
osteoinductive growth factors have been used for
generation of vascularized bone tissues in combi-
nation with a vascular axis or vascularized flaps.
Revascularization of scaffolds is induced by an
inflammatory wound healing response as a reaction
to the surgical implantation. This, combined with
the hypoxia within the implant evokes local
expression of angiogenetic growth factors. Bone
formation beneath “standard flaps” has been suc-
cessfully induced using bioceramics seeded with
autologous bone marrow stromal cells .
Induction of axial vascularization protected porous
biomaterials from bacterial infection and transfer
of this vascularized hard tissue as a free flap has
been demonstrated . Pedicled bone flaps
based on collagen I scaffolds, bone marrow stro-
mal cells and a PTFE membrane have been suc-
cessfully generated using the carotid artery and
jugular vein or the saphenous bundle as vascular
axis . Prefabricated vascularized bone grafts
have even be used in a clinical setting for mandibu-
lar reconstruction following thorough in vivo eval-
uation in a pig model. This group buried granules
of xenogenic bone minerals soaked with recombi-
nant OP-1 in the latissimus dorsi muscle and trans-
ferred the neo-tissue using microsurgical tech-
niques into mandibular defects [129, 130]. In the
clinical setting a titanium cage was custom made
according to CT scan and 3D reconstruction data,
filled with bone marrow aspirate, xenogenic bone
minerals and OP-1, and a large mandibular defect
was successfully reconstructed following a prefab-
rication period of 7 weeks .
“Free-Style” vascularized bioartificial bone
In the last decade the field of surgically induced angio-
genesis has tremendously developed. Induction of
“intrinsic” vascularization in biomaterials allowed the
generation of vascularized tissues at different sites for
transfer as pedicled or free flaps in several animal
models.Although a number of vascular axes are avail-
able for intrinsically vascularized tissue compounds in
humans, there remain limitations with regard to pedi-
cle length and anatomic location. The creation of a
vascular axis using vein grafts holds promise for gen-
eration of vascularized bone units relatively indepen-
dent of anatomical limitations. Erol and Spira man-
aged to produce a prefabricated skin flap by means of
an arteriovenous vessel - loop using either artery or
vein grafts in a rat model . They observed an
J. Cell. Mol. Med. Vol 10, No 1, 2006
abundant neovascular outgrowth originating from the
entire AV Loop. Morrison and co-workers augmented
this model and implanted the AV-loop into polycar-
bonate isolation chambers. Furthermore they induced
vascularization in polymer matrices and managed to
generate large volumes of axially vascularized tissue
[133–135]. In the era of tissue engineering this con-
cept met with great interest. Recently, our group vas-
cularized successfully a custom-made processed
bovine cancellous bone matrix by means of an arteri-
ovenous loop . Meticulous analysis of the angio-
genetic response by morphometry, high resolution
Fig. 1 Vascularization of porous matrices by implanting an arteriovenous loop. A. The arteriovenous loop consist-
ing of an isolated artery and vein, and a vein graft of variable length is constructed using microsurgical techniques.
In the rat model the loop is constructed between the femoral artery and vein. B. The significant degree of vascular-
ity in the axially vascularized bioartificial tissue is demonstrated by intravital MRI angiography. High flow rates are
highlighted by yellow staining. C&D. Differentiated morphology of the vascular system originating from the arte-
riovenous loop is demonstrated by sanning electron microscopy of vascular corrosion replicas. Vessels of different
calibers invade the porous matrix and form a vascular bed for subsequent injection of osteogenic cells.
micro MRI and vascular corrosion casts revealed a
vascularization of more than 90% of the scaffold with-
in 8 weeks following implantation [Fig. 1]. The
amount of vascularization was comparable with
extrinsically vascularized control matrices; however,
the inflammatory reaction was considerably less pro-
nounced in the AV loop group . Furthermore,
prevascularization of porous hard tissue scaffolds by
means of an arteriovenous loop significantly increased
the number of initially engrafted osteoblasts in prelim-
inary experiments . Bone formation following
osteoblast injection is right now being evaluated over
a longer observation period in the same model.
Tissue engineering is a fascinating field of research and
is bound to dramatically change clinical practice in
reconstructive surgery. Osteogenic cells for bioactive
implants are readily available following minimally
invasive harvesting and ex vivo expansion. A plethora
of highly innovative biomaterials with well tuned
matrix properties have been developed to perfectly
meet the clinician’s requirements. Osteoinductive sub-
stances may further enhance bone formation within
engineered composites. Optimized implantation tech-
niques are one more essential step towards clinical
application of engineered bioartificial bone tissues.The
answers towards upscaling of bioartificial devices will
be delivered by advances in the area of vascularization.
In the future, joint approaches are needed in order to
transfer highly potent bioartificial osteogenic bone tis-
sues into the demanding in vivo environment [Fig. 2].
Close cooperation between tissue engineers and recon-
structive surgeons may eventually help to bridge the
gap between bench and bedside.
The authors would like to thank Dr. A. Hess for the micro
MRI angiography and Dr. T. Fey for the ESM pictures.
1. Buckwalter JA, Glimcher MJ, Cooper RR, Recker R.
Bone biology. II: Formation, form, modeling, remodeling,
and regulation of cell function. Instr Course Lect. 1996; 45:
2. Buckwalter JA, Glimcher MJ, Cooper RR, Recker R.
Bone biology. I: Structure, blood supply, cells, matrix, and
mineralization. Instr Course Lect. 1996; 45: 371–86,.
3. Ackerman LV, Spjut HJ, Abell MR, Bones and Joints
(Monographs in Pathology). Baltimore: Williams and
4. Aubin JE. Bone stem cells. J Cell Biochem Suppl 1998; 30-
5. Owen M. The origin of bone cells. Int Rev Cytol. 1970; 28:
6. Heinegard D, Oldberg A. Structure and biology of cartilage
and bone matrix noncollagenous macromolecules. FASEB J
1989; 3: 2042–51.
7. Robey PG, Fedarko NS, Hefferan TE, Bianco P, Vetter
UK, Grzesik W, Friedenstein A, Van der PG, Mintz KP,
Young MF. Structure and molecular regulation of bone
matrix proteins. J Bone Miner Res. 1993; 2: S483–7.
8. Huang S, Ingber DE. The structural and mechanical com-
plexity of cell-growth control. Nat Cell Biol. 1999; 1:
9. Lian JB, Stein GS. Development of the osteoblast pheno-
type: molecular mechanisms mediating osteoblast growth
and differentiation. Iowa Orthop J. 1995; 15: 118–40.
10. Nomura S, Takano-Yamamoto T. Molecular events caused
by mechanical stress in bone. Matrix Biol. 2000; 19: 91-6.
11. Probst A, Spiegel HU. Cellular mechanisms of bone repair.
J Invest Surg. 1997; 10: 77–86.
J. Cell. Mol. Med. Vol 10, No 1, 2006
Fig. 2 Joint approaches are needed for efficient trans-
fer of larger volume bone implants.
12. Olsen BR, Reginato AM, Wang W. Bone development.
Annu Rev Cell Dev Biol. 2000; 16: 191–220.
13. Stein GS, Lian JB, Owen TA. Relationship of cell growth
to the regulation of tissuespecific gene expression during
osteoblast differentiation, FASEB J. 1990; 4: 3111–23.
14. Mundy GR. Regulation of bone formation by bone mor-
phogenetic proteins and other growth factors, Clin Orthop
Relat Res. 1996; 324: 24–8.
15. Stein GS, Lian JB, Stein JL, Van Wijnen AJ, Montecino
M. Transcriptional control of osteoblast growth and differ-
entiation. Physiol Rev. 1996; 76: 593–629.
16. Ducy P, Karsenty G. Genetic control of cell differentiation
in the skeleton. Curr Opin Cell Biol. 1998; 10: 614–9.
17. Reddi AH. Initiation of fracture repair by bone morpho-
genetic proteins. Clin Orthop Relat Res. 1998; 355: S66–72.
18. Ducy P. Cbfa1: a molecular switch in osteoblast biology.
Dev Dyn. 2000; 219: 461–71.
19. Karsenty G. Minireview: transcriptional control of
osteoblast differentiation. Endocrinology 2001; 142:
20. Urist MR, DeLange RJ, Finerman GA. Bone cell differ-
entiation and growth factors. Science 1983; 13,220: 680–6.
21. Lieberman JR, Daluiski A, Einhorn TA. The role of
growth factors in the repair of bone. Biology and clinical
applications. J Bone Joint Surg Am. 2002; 84-A: 1032–44.
22. Perry CR. Bone repair techniques, bone graft, and bone
graft substitutes. Clin Orthop Relat Res. 1999; 360: 71–86.
23. Gugenheim JJ Jr. The Ilizarov method. Orthopedic and soft
tissue applications, Clin Plast Surg. 1998; 25: 567–78.
24. Motoki DS, Mulliken JB. The healing of bone and carti-
lage. Clin Plast Surg. 1990; 17: 527–44.
25. Polykandriotis E, Stangl R, Hennig HH, Lennerz JK,
Frank WM, Loos MD, Horch RE. The composite vastus
medialis-patellar complex osseomuscular flap as a salvage
procedure after complex trauma of the knee—an anatomical
study and clinical application. Br J Plast Surg. 2005; 58:
26. Gazdag AR, Lane JM, Glaser D, Forster RA.Alternatives
to autogenous bone graft: efficacy and indications. J Am
Acad Orthop Surg. 1995; 3: 1–8.
27. Sassard WR, Eidman DK, Gray PM, Block JE, Russo R,
Russell JL, Taboada EM. Augmenting local bone with
Grafton demineralized bone matrix for posterolateral lumbar
spine fusion: avoiding second site autologous bone harvest,
Orthopedics 2000; 23: 1059–64.
28. Arrington ED, Smith WJ, Chambers HG, Bucknell AL,
Davino NA. Complications of iliac crest bone graft harvest-
ing. Clin Orthop Relat Res. 1996; 329: 300–9.
29. Banwart JC, Asher MA, Hassanein RS. Iliac crest bone
graft harvest donor site morbidity. A statistical evaluation.
Spine 1995; 1,20: 1055–60.
30. Ebraheim NA, Elgafy H, Xu R. Bone-graft harvesting
from iliac and fibular donor sites: techniques and complica-
tions. J Am Acad Orthop Surg. 2001; 9: 210–8.
31. Lobo Gajiwala A, Agarwal M, Puri A, D’Lima C, Duggal
A. Reconstructing tumour defects: lyophilised, irradiated
bone allografts. Cell Tissue Bank 4: 109–18, 2003.
32. Aho AJ, Ekfors T, Dean PB, Aro HT, Ahonen A,
Nikkanen V. Incorporation and clinical results of large allo-
grafts of the extremities and pelvis. Clin Orthop Relat Res.
1994; 307: 200–13.
33. Cetiner S, Esen E, Ustun Y, Oztunc H, Tuncer I. Long-
term results of the application of solvent-dehydrated bone
xenograft and duramater xenograft for the healing of
oroantral osseous defects: a pilot experimental study. Dent
Traumatol. 2003; 19: 30–5.
34. Swartz WM, Banis JC, Newton ED, Ramasastry SS,
Jones NF, Acland R. The osteocutaneous scapular flap for
mandibular and maxillary reconstruction. Plast Reconstr
Surg. 1986; 77: 530–45.
35. Shea KG, Coleman DA, Scott SM, Coleman SS,
Christianson M. Microvascularized free fibular grafts for
reconstruction of skeletal defects after tumor resection. J
Pediatr Orthop. 1997; 17: 424–32.
36. Ozaki T, Hillmann A, Wuisman P, Winkelmann W.
Reconstruction of tibia by ipsilateral vascularized fibula and
allograft. 12 cases with malignant bone tumors. Acta Orthop
Scand. 1997; 68: 298–301.
37. Babovic S, Johnson CH, Finical SJ. Free fibula donor-site
morbidity: the Mayo experience with 100 consecutive har-
vests. J Reconstr Microsurg. 2000; 16: 107–10.
38. Lewis G. Properties of acrylic bone cement: state of the art
review, J Biomed Mater Res. 1997; 2: 155–82.
39. Muh E, Zimmermann J, Kneser U, Marquardt J,
Mulhaupt R, Stark B. Lysineurethanedimethacrylate—a
novel generation of amino acid based monomers for bone
cements and tissue repair. Biomaterials 2002; 23: 2849–54.
40. Zijderveld SA, Zerbo IR, van den Bergh JP, Schulten
EA, ten Bruggenkate CM. Maxillary sinus floor augmen-
tation using a beta-tricalcium phosphate (Cerasorb) alone
compared to autogenous bone grafts. Int J Oral Maxillofac
Implants. 2005;20: 432–40.
41. Cassidy C, Jupiter JB, Cohen M, Delli-Santi M, Fennell
C, Leinberry C, Husband J, Ladd A, Seitz WR, Constanz
B. Norian SRS cement compared with conventional fixation
in distal radial fractures. A randomized study. J Bone Joint
Surg Am. 2003;85-A: 2127–37.
42. Jupiter JB, Winters S, Sigman S, Lowe C, Pappas C,
Ladd AL, Van Wagoner M, Smith ST. Repair of five dis-
tal radius fractures with an investigational cancellous bone
cement: a preliminary report. J Orthop Trauma. 1997; 11:
43. Thorwarth M, Wehrhan F, Schultze-Mosgau S, Wiltfang
J, Schlegel KA. PRP modulates expression of bone matrix
proteins in vivo without long-term effects on bone forma-
tion. Bone 2006; 38: 30–40.
44. Sammartino G, Tia M, Marenzi G, di Lauro AE,
D’Agostino E, Claudio PP. Use of autologous platelet-rich
plasma (PRP) in periodontal defect treatment after extraction
of impacted mandibular third molars. J Oral Maxillofac
Surg. 2005; 63: 766–70.
45. Altmeppen J, Hansen E, Bonnlander GL, Horch RE,
Jeschke MG. Composition and characteristics of an autolo-
gous thrombocyte gel. J Surg Res. 2004; 117: 202–7.
46. Moghadam HG, Sandor GK, Holmes HH, Clokie CM,
Histomorphometric evaluation of bone regeneration using
allogeneic and alloplastic bone substitutes. J Oral Maxillofac
Surg. 2004; 62: 202–13.
47. Maddox E, Zhan M, Mundy GR, Drohan WN, Burgess
WH. Optimizing human demineralized bone matrix for clin-
ical application. Tissue Eng. 2000; 6: 441–8.
48. Traianedes K, Russell JL, Edwards JT, Stubbs HA,
Shanahan IR, Knaack D. Donor age and gender effects on
osteoinductivity of demineralized bone matrix. J Biomed
Mater Res B Appl Biomater. 2004; 70: 21–9.
49. Pietrzak WS, Perns SV, Keyes J, Woodell-May J,
McDonald NM. Demineralized bone matrix graft: a scien-
tific and clinical case study assessment. J Foot Ankle Surg.
2005; 44: 345–53.
50. Andreana S, Cornelini R, Edsberg LE, Natiella JR,
Maxillary sinus elevation for implant placement using calci-
um sulfate with and without DFDBA: six cases. Implant
Dent. 2004; 13: 270–7.
51. Reddi AH. Role of morphogenetic proteins in skeletal tissue
engineering and regeneration. Nat Biotechnol. 1998; 16:
52. Einhorn TA. Clinical applications of recombinant human
BMPs: early experience and future development. J Bone
Joint Surg Am. 2003; 85-A: 82–8.
53. Kain MS, Einhorn TA. Recombinant human bone morpho-
genetic proteins in the treatment of fractures. Foot Ankle
Clin. 2005; 4: 639–50.
54. Dimitriou R, Dahabreh Z, Katsoulis E, Matthews SJ,
Branfoot T, Giannoudis PV. Application of recombinant
BMP-7 on persistent upper and lower limb nonunions, Injury
2005; 36: S51–9.
55. Govender S, Csimma C, Genant HK, Valentin-Opran A,
Amit Y, Arbel R, Aro H, Atar D, Bishay M, Borner MG,
Chiron P, Choong P, Cinats J, Courtenay B, Feibel R,
Geulette B, Gravel C, Haas N, Raschke M, Hammacher
E, van der Velde D, Hardy P, Holt M, Josten C, Ketterl
RL, Lindeque B, Lob G, Mathevon H, McCoy G, Marsh
D, Miller R, Munting E, Oevre S, Nordsletten L, Patel A,
Pohl A, Rennie W, Reynders P, Rommens PM, Rondia J,
Rossouw WC, Daneel PJ, Ruff S, Ruter A, Santavirta S,
Schildhauer TA, Gekle C, Schnettler R, Segal D, Seiler H,
Snowdowne RB, Stapert J, Taglang G, Verdonk R, Vogels
L, Weckbach A, Wentzensen A, Wisniewski T; BMP-2
Evaluation in Surgery for Tibial Trauma (BESTT) Study
Group. Recombinant human bone morphogenetic protein-2
for treatment of open tibial fractures: a prospective, con-
trolled, randomized study of four hundred and fifty patients.
J Bone Joint Surg Am. 2002; 84-A: 2123–34.
56. Langer R, Vacanti JP. Tissue engineering. Science 1993;
57. Kneser U, Kaufmann PM, Fiegel HC, Pollok JM, Kluth
D, Herbst H, Rogiers X. Long-term differentiated function
of heterotopically transplanted hepatocytes on threedimen-
sional polymer matrices. J Biomed Mater Res. 1999; 47:
58. Kneser U, Schaefer DJ, Munder B, Klemt C, Andree C,
Stark GB. Tissue engineering of bone. Min Invas Sur &
Allied Technol. 2002; 3: 107–16.
59. Vacanti CA, Vacanti JP. Bone and cartilage reconstruction
with tissue engineering approaches. Otolaryngol Clin North
Am. 1994; 27: 263–76.
60. Stock UA, Vacanti JP. Tissue engineering: current state and
prospects. Annu Rev Med. 2001; 52: 443–51.
61. Bach AD, Beier JP, Stern-Staeter J, Horch RE. Skeletal
muscle tissue engineering, J Cell Mol Med. 2004; 8: 413–22.
62. Horch RE, Kopp J, Kneser U, Beier J, Bach AD, Tissue
engineering of cultured skin substitutes. J Cell Mol Med.
2005; 9: 592–608.
63. Cornell CN, Lane JM. Current understanding of osteocon-
duction in bone regeneration. Clin Orthop Relat Res. 1998;
64. Hotz G, Herr G. Bone substitute with osteoinductive bio-
materials - current and future clinical applications. Int J Oral
Maxillofac Surg. 1994; 23: 413–7.
65. Cooper LF, Harris CT, Bruder SP, Kowalski R, Kadiyala
S. Incipient analysis of mesenchymal stem-cell-derived
osteogenesis. J Dent Res. 2001; 80: 314–20.
66. Shin H, Jo S, Mikos AG. Biomimetic materials for tissue
engineering. Biomaterials 2003; 24: 4353–64.
67. Yang S, Leong KF, Du Z, Chua CK. The design of scaf-
folds for use in tissue engineering. Part I. Traditional factors.
Tissue Eng. 2002; 8: 1–11.
68. Logeart-Avramoglou D, Anagnostou F, Bizios R, Petite
H. Engineering bone: challenges and obstacles. J Cell Mol
Med. 2005; 9: 72–84.
69. Kneser U, Voogd A, Ohnolz J, Buettner O, Stangenberg
L, Zhang YH, Stark GB, Schaefer DJ. Fibrin gel-immobi-
lized primary osteoblasts in calcium phosphate bone cement:
in vivo evaluation with regard to application as injectable
biological bone substitute. Cells Tissues Organs. 2005; 179:
70. Schantz JT, Teoh SH, Lim TC, Endres M, Lam CX,
Hutmacher DW. Repair of calvarial defects with cus-
tomized tissue-engineered bone grafts I. Evaluation of osteo-
genesis in a three-dimensional culture system. Tissue Eng.
2003; 9: S113–26.
71. Petite H, Viateau V, Bensaid W, Meunier A, de Pollak C,
Bourguignon M, Oudina K, Sedel L, Guillemin G.
Tissue-engineered bone regeneration. Nat Biotechnol. 2000;
72. Mankani MH, Kuznetsov SA, Fowler B, Kingman A,
Robey PG. In vivo bone formation by human bone marrow
stromal cells: effect of carrier particle size and shape,
Biotechnol Bioeng. 2001; 72: 96–107.
73. Sikavitsas VI, van den Dolder J, Bancroft GN, Jansen
JA, Mikos AG. Influence of the in vitro culture period on the
in vivo performance of cell/titanium bone tissueengineered
constructs using a rat cranial critical size defect model. J
Biomed Mater Res A. 2003; 67: 944–51.
74. Timmer MD, Shin H, Horch RA, Ambrose CG, Mikos
AG. In Vitro cytotoxicity of injectable and biodegradable
poly(propylene fumarate)-based networks: unreacted
macromers, cross-linked networks, and degradation prod-
ucts. Biomacromolecules 2003; 4: 1026–33.
75. Stangenberg L, Schaefer DJ, Buettner O, Ohnolz J,
Moebest D, Horch RE, Stark GB, Kneser U,
Differentiation of osteoblasts in three-dimensional culture in
porous cancellous bone matrix: quantitative analysis of gene
expression based on real-time reverse transcription poly-
merase chain reaction. Tissue Eng. 2005; 11: 855–64.
76. Groger A, Klaring S, Merten HA, Holste J, Kaps C,
Sittinger M. Tissue engineering of bone for mandibular aug-
mentation in immunocompetent minipigs: preliminary study.
Scand J Plast Reconstr Surg Hand Surg. 2003; 37: 129–33.
77. Schantz JT, Hutmacher DW, Lam CX, Brinkmann M,
J. Cell. Mol. Med. Vol 10, No 1, 2006
Wong KM, Lim TC, Chou N, Guldberg RE, Teoh SH.
Repair of calvarial defects with customised tissueengineered
bone grafts II. Evaluation of cellular efficiency and efficacy
in vivo. Tissue Eng. 2003; 9: S127–39.
78. Yang S, Leong KF, Du Z, Chua CK, The design of scaf-
folds for use in tissue engineering. Part II. Rapid prototyping
techniques. Tissue Eng. 2001; 7: 679–89.
79. Bruder SP, Fox BS. Tissue engineering of bone. Cell based
strategies. Clin Orthop Relat Res. 1999; 367: S68–83.
80. Bruder SP, Caplan AI. Terminal differentiation of
osteogenic cells in the embryonic chick tibia is revealed by a
monoclonal antibody against osteocytes. Bone 1990; 11:
81. Bruder SP, Fink DJ, Caplan AI. Mesenchymal stem cells
in bone development, bone repair, and skeletal regeneration
therapy. J Cell Biochem. 1994; 56: 283–94.
82. Aubin JE. Advances in the osteoblast lineage. Biochem Cell
Biol. 1998; 76: 899–910.
83. Kuznetsov SA, Krebsbach PH, Satomura K, Kerr J,
Riminucci M, Benayahu D, Robey PG. Single-colony
derived strains of human marrow stromal fibroblasts form
bone after transplantation in vivo. J Bone Miner Res. 1997;
84. Vacanti CA, Bonassar LJ, Vacanti MP, Shufflebarger J.
Replacement of an avulsed phalanx with tissue-engineered
bone. N Engl J Med. 2001; 344: 1511–4.
85. Hentz VR, Chang J. Tissue engineering for reconstruction
of the thumb. N Engl J Med. 2001; 344: 1547–8.
86. Ueda M, Yamada Y, Ozawa R, Okazaki Y. Clinical case
reports of injectable tissueengineered bone for alveolar aug-
mentation with simultaneous implant placement. Int J
Periodontics Restorative Dent. 2005; 25: 129–37.
87. Schmelzeisen R, Schimming R, Sittinger M. Making
bone: implant insertion into tissue-engineered bone for max-
illary sinus floor augmentation-a preliminary report. J
Craniomaxillofac Surg. 2003; 31: 34–9.
88. Schimming R, Schmelzeisen R. Tissue-engineered bone for
maxillary sinus augmentation. J Oral Maxillofac Surg. 2004;
89. Reddi AH. Morphogenesis and tissue engineering of bone
and cartilage: inductive signals, stem cells, and biomimetic
biomaterials. Tissue Eng. 2000; 6: 351–9.
90. Reddi AH. Regulation of cartilage and bone differentiation
by bone morphogenetic proteins. Curr Opin Cell Biol. 1992;
91. Hollinger JO, Uludag H, Winn SR, Sustained release
emphasizing recombinant human bone morphogenetic pro-
tein-2. Adv Drug Deliv Rev. 1998;31: 303–18.
92. Musgrave DS, Bosch P, Lee JY, Pelinkovic D, Ghivizzani
SC, Whalen J, Niyibizi C, Huard J, Ex vivo gene therapy
to produce bone using different cell types. Clin Orthop Relat
Res. 2000; 378: 290–305.
93. Salyapongse AN, Billiar TR, Edington H, Gene therapy
and tissue engineering. Clin Plast Surg. 1999; 26: 663–76.
94. Wu D, Razzano P, Grande DA. Gene therapy and tissue
engineering in repair of the musculoskeletal system. J Cell
Biochem. 2003; 88: 467–81.
95. Luo J, Sun MH, Kang Q, Peng Y, Jiang W, Luu HH, Luo
Q, Park JY, Li Y, Haydon RC, He TC. Gene therapy for
bone regeneration. Curr Gene Ther. 2005; 5: 167–79.
96. Chang SC, Chuang H, Chen YR, Yang LC, Chen JK,
Mardini S, Chung HY, Lu YL, Ma WC, Lou J. Cranial
repair using BMP-2 gene engineered bone marrow stromal
cells. J Surg Res. 2004; 119: 85–91.
97. Nakashima S, Matsuyama Y, Nitta A, Sakai Y, Ishiguro
N. Highly efficient transfection of human marrow stromal
cells by nucleofection. Transplant Proc. 2005; 37: 2290–2.
98. Bonadio J, Smiley E, Patil P, Goldstein S. Localized, direct
plasmid gene delivery in vivo: prolonged therapy results in
reproducible tissue regeneration. Nat Med. 1999; 5: 753–9.
99. Goldstein AS, Juarez TM, Helmke CD, Gustin MC,
Mikos AG. Effect of convection on osteoblastic cell growth
and function in biodegradable polymer foam scaffolds.
Biomaterials 2001; 22: 1279–88.
100. Folkman J, Hochberg M. Self-regulation of growth in three
dimensions. J Exp Med. 1973; 138: 745–53.
101. Kneser U, Stangenberg L, Ohnolz J, Buettner O, Stern-
Strater J, Moebest D, Horch RE, Stark GB, Schaefer DJ.
Reconstruction of critical size calvarial defects using pro-
cessed bovine cancellous bone matrix and autologous
osteoblasts. J Cell Mol Med. submitted: 2006.
102. Sottile J. Regulation of angiogenesis by extracellular matrix.
Biochim Biophys Acta. 2004; 1654: 13–22.
103. Madeddu P, Therapeutic angiogenesis and vasculogenesis
for tissue regeneration. Exp Physiol. 2005; 90: 315–26.
104. Byrne AM, Bouchier-Hayes DJ, Harmey JH. Angiogenic
and cell survival functions of vascular endothelial growth
factor (VEGF). J Cell Mol Med. 2005; 9: 777–94.
105. Tabata Y. Tissue regeneration based on growth factor
release. Tissue Eng. 2003; 9: S5–15.
106. Elcin YM, Dixit V, Gitnick G. Extensive in vivo angiogen-
esis following controlled release of human vascular endothe-
lial cell growth factor: implications for tissue engineering
and wound healing. Artif Organs. 2001; 25: 558–65.
107. Ahrendt G, Chickering DE, Ranieri JP. Angiogenic
growth factors: a review for tissue engineering. Tissue Eng.
1998; 2: 117–30.
108. Wong C, Inman E, Spaethe R, Helgerson S. Fibrin-based
biomaterials to deliver human growth factors. Thromb
Haemost. 2003; 89: 573–82.
109. Sakiyama-Elbert SE, Hubbell JA. Development of fibrin
derivatives for controlled release of heparin- binding growth
factors. J Control Release. 2000; 65: 389–402.
110. Wenger A, Stahl A, Weber H, Finkenzeller G, Augustin
HG, Stark GB, Kneser U. Modulation of in vitro angiogen-
esis in a three-dimensional spheroidal coculture model for
bone tissue engineering. Tissue Eng. 2004; 10: 1536–47.
111. Mertsching H, Walles T, Hofmann M, Schanz J, Knapp
WH. Engineering of a vascularized scaffold for artificial tis-
sue and organ generation. Biomaterials 2005; 26: 6610–7.
112. Niklason LE, Gao J, Abbott WM, Hirschi KK, Houser S,
Marini R, Langer R. Functional arteries grown in vitro.
Science 1999; 284: 489–93.
113. Tremblay PL, Hudon V, Berthod F, Germain L, Auger
FA. Inosculation of tissueengineered capillaries with the
host’s vasculature in a reconstructed skin transplanted on
mice. Am J Transplant. 2005; 5: 1002–10.
114. Mooney DJ, Mikos AG. Growing new organs. Sci Am.
1999; 4: 60–5.
115. Eiselt P, Kim BS, Chacko B, Isenberg B, Peters MC,
Greene KG, Roland WD, Loebsack AB, Burg KJ,
Culberson C, Halberstadt CR, Holder WD, Mooney DJ.
Development of technologies aiding large-tissue engineer-
ing. Biotechnol Prog. 1998; 14: 134–40.
116. Cassell OC, Hofer SO, Morrison WA, Knight KR.
Vascularisation of tissueengineered grafts: the regulation of
angiogenesis in reconstructive surgery and in disease states.
Br J Plast Surg. 2002; 55: 603–10.
117. Beier JP, Kneser U, Stern-Strater J, Stark GB, Bach AD.
Y chromosome detection of three-dimensional tissue-engi-
neered skeletal muscle constructs in a syngeneic rat animal
model. Cell Transplant. 2004; 13: 45–53.
118. Schipper J, Ridder GJ, Maier W, Horch RE. The precon-
ditioning and prelamination of pedicled and free microvas-
cular anastomised flaps with the technique of vacuum assist-
ed closure. Laryngorhinootologie 2003; 82: 421–7.
119. Khouri RK, Upton J, Shaw WW. Principles of flap pre-
fabrication. Clin Plast Surg. 1992; 19: 763–71.
120. Kimura N, Hasumi T, Satoh K. Prefabricated thin flap
using the transversalis fascia as a carrier. Plast Reconstr
Surg. 2001; 108: 1972–80.
121. Khouri RK, Upton J, Shaw WW. Prefabrication of com-
posite free flaps through staged microvascular transfer: an
experimental and clinical study. Plast Reconstr Surg. 1991;
122. Abbase EA, Shenaq SM, Spira M, el-Falaky MH.
Prefabricated flaps: experimental and clinical review. Plast
Reconstr Surg. 1995; 96: 1218–25.
123. Gill DR, Ireland DC, Hurley JV, Morrison WA. The pre-
fabrication of a bone graft in a rat model. J Hand Surg [Am].
1998; 23: 312–21.
124. Homma K, Himi T, Hoki K, Ezoe K, Shintani T,
Yamaguchi H, Fujita T, A prefabricated osteocutaneous
flap for tracheal reconstruction. Plast Reconstr Surg. 2003;
125. Safak T, Akyurek M, Ozcan G, Kecik A, Aydin M.
Osteocutaneous flap prefabrication based on the principle of
vascular induction: an experimental and clinical study. Plast
Reconstr Surg. 2000;105: 1304–13.
126. Casabona F, Martin I, Muraglia A, Berrino P, Santi P,
Cancedda R, Quarto R. Prefabricated engineered bone
flaps: an experimental model of tissue reconstruction in plas-
tic surgery. Plast Reconstr Surg. 1998; 3: 577–81.
127. Bernard SL, Picha GJ. The use of coralline hydroxyapatite
in a “biocomposite” free flap. Plast Reconstr Surg. 1991; 87:
128. Mankani MH, Krebsbach PH, Satomura K, Kuznetsov
SA, Hoyt R, Robey PG. Pedicled bone flap formation using
transplanted bone marrow stromal cells. Arch Surg. 2001;
129. Terheyden H, Warnke P, Dunsche A, Jepsen S, Brenner
W, Palmie S, Toth C, Rueger DR. Mandibular reconstruc-
tion with prefabricated vascularized bone grafts using
recombinant human osteogenic protein-1: an experimental
study in miniature pigs. Part II: transplantation. Int J Oral
Maxillofac Surg. 2001; 30: 469–78.
130. Terheyden H, Menzel C, Wang H, Springer IN, Rueger
DR, Acil Y. Prefabrication of vascularized bone grafts using
recombinant human osteogenic protein-1 - part 3: dosage of
rhOP-1, the use of external and internal scaffolds. Int J Oral
Maxillofac Surg. 2004; 33: 164–72.
131. Warnke PH, Springer IN, Wiltfang J, Acil Y, Eufinger H,
Wehmoller M, Russo PA, Bolte H, Sherry E, Behrens E,
Terheyden H. Growth and transplantation of a custom vas-
cularised bone graft in a man. Lancet 2004; 364: 766–70.
132. Erol OO, Spira M. New capillary bed formation with a sur-
gically constructed arteriovenous fistula. Surg Forum. 1979;
133. Mian R, Morrison WA, Hurley JV, Penington AJ, Romeo
R, Tanaka Y, Knight KR. Formation of new tissue from an
arteriovenous loop in the absence of added extracellular
matrix. Tissue Eng. 2000; 6: 595–603.
134. Hofer SO, Knight KM, Cooper-White JJ, O’Connor AJ,
Perera JM, Romeo-Meeuw R, Penington AJ, Knight KR,
Morrison WA, Messina A. Increasing the volume of vascu-
larized tissue formation in engineered constructs: an experi-
mental study in rats. Plast Reconstr Surg. 2003; 3: 1186–92.
135. Cassell OC, Morrison WA, Messina A, Penington AJ,
Thompson EW, Stevens GW, Perera JM, Kleinman HK,
Hurley JV, Romeo R, Knight KR. The influence of extra-
cellular matrix on the generation of vascularized, engineered,
transplantable tissue. Ann N Y Acad Sci. 2001; 944: 429–42.
136. Kneser U, Polykandriotis E, Ohnolz J, Heidner K,
Grabinger L, Euler S, Aman KU, Hess A, Brune K, Greil
P, Sturzl M, Horch RE. Engineering of vascularized trans-
plantable bone tissues: induction of axial vascularization in
an osteconductive matrix using an arteriovenous loop. Tissue
Eng. in press. 2006.
137. Polykandriotis E, Horch RE, Arkudas A, Labanaris A,
Brune K, Greil P, Bach AD, Kopp J, Hess A, Kneser U.
Intrinsic versus extrinsic vascularization in tissue engineer-
ing. Adv Mol Biol Med. in press. 2006.
138. Kneser U, Arkudas A, Polykandriotis E, Heidner K,
Ohnolz J, Beier JP, Bach AD, Kopp J, Hess A, Horch
RE. Axial prevascularization of porous matrices by means
of an arteriovenous loop significantly increases initial sur-
vival of transplanted autologous osteoblasts. Tissue Eng.
J. Cell. Mol. Med. Vol 10, No 1, 2006